International Journal of
Characteristics of LiNi1/3
Prepared by Different Method in Lithium Rechargeable
Sung-Keun Kim1, Woon-Tae Jeong2, Hong-Ki Lee3, Joongpyo Shim1,*
1 Department of Chemical Engineering, Kunsan National University, Jeonbuk, 573-701, Korea 2 Umicore Korea Ltd, Chungnam, 330-200, Korea
3 Fuel Cell Regional Innovation Center, Woosuk University, Jeonbuk, 565-701, Korea *E-mail: firstname.lastname@example.org
Received: 1 September 2008 / Accepted: 25 October 2008 / Published: 17 November 2008
LiNi1/3Co1/3Mn1/3O2 materials were synthesized by different synthetic routes; through spray-drying, combustion, or solid-state reactions. The LiNi1/3Co1/3Mn1/3O2 powders were examined by X-ray diffraction (XRD), scanning electron microscopy (SEM), particle size analysis, and charge/discharge cycling. All the prepared LiNi1/3Co1/3Mn1/3O2 powders were identified as hexagonal structures and exhibited discharge capacities of ca. 130-140 mAh/g at 2.8-4.3 V. The LiNi1/3Co1/3Mn1/3O2 powder prepared through the spray-drying method showed better electrochemical properties, such as discharge capacity, rate capability, and constant cycling, over those synthesized from combustion and solid-state reaction.
Keywords: Lithium-ion batteries, spray-drying, cathode, LiNi1/3Co1/3Mn1/3O2, combustion
Rechargeable lithium-ion batteries have been developed and LiCoO2 has been widely used as cathode material because of its high cycleability.  However, its capacity is limited due to a structural change above 4.3V and cobalt is relatively expensive and toxic compared to nickel, manganese and iron which can form various layered oxides with lithium. Many researchers have tried to develop low cost and less toxic materials such as nickel (LiNiO2), manganese (LiMn2O4 or LiMnO2) and iron (LiFePO4)-based materials.
relatively low cost compared to layered oxides such as LiCoO2.  LiNi1/3Co1/3Mn1/3O2 has been prepared by a solid-state reaction which has several disadvantages, such as inhomogeneous composition, irregular morphology, large particle size, and long heating times followed by several grinding and annealing processes.  In this work, we report on the synthesis and electrochemical characteristics of LiNi1/3Co1/3Mn1/3O2 materials prepared from three different methods; spray-drying, combustion and solid-state reaction.
2. EXPERIMENTAL PART
For the spray-drying (SD) method, the LiNi1/3Co1/3Mn1/3O2 precursors were prepared using LiCH3COO·2H2O, Ni(CH3COO)2·4H2O, Co(CH3COO)2·4H2O, Mn(CH3COO)2·4H2O with a molar ratio of Li/Me = 1.1 (Me=Ni, Co and Mn). These metal acetates were dissolved in deionized water. The resulting solution was sprayed to form a homogeneous mixture of precursors at 150oC. The mixed precursor powder was heated to 400oC for 4 h in air. Then the obtained powder was ground in a mortar and re-annealed at 900oC for 15 h in air. 
For the combustion method (CB), Li(NO3)2·4H2O, Ni(CH3COO)2·4H2O, Co(CH3COO)2·4H2O, and Mn(CH3COO)2·4H2O were dissolved in deionized water with a molar ratio of Li/Me = 1.1 (Me=Ni, Co and Mn). The dissolved solution was heated at 80-90oC to make a green-colored gel. It was then burned and transformed into a black sponge-like fluffy material. The powder was additionally sintered at 900oC for 15 h.
LiNi1/3Co1/3Mn1/3O2 materials were prepared by the solid-state reaction (SS) of precursors. The precursors were prepared in the same manner as in the spray-drying method above. The metal acetate precursors were well-mixed in a mortar and pressed into pellet. The pellet was preheated at 400oC in air for 4 h and then sintered at 900oC for 15 h.
The thermo gravimetric analysis (TGA) for the mixture of precursors was conducted in air atmosphere to observe the temperature for precursor decomposition and calcination. The LiNi1/3Co1/3Mn1/3O2 powders were characterized by X-ray diffraction (XRD) using an X-ray diffractometer (Bruker M18XCE) with Cu-Kα radiation. The particle morphology and size distribution were observed by scanning electron microscopy (SEM) and a particle size analyzer (Analysette 22, Fritsch).
3. RESULTS AND DISCUSSION
The temperature for the decomposition of precursors, metal acetates containing lithium, nickel, manganese and cobalt, was observed using by thermo-gravimetric analysis (TGA), as shown in Fig. 1. Most of hydrate in precursor was vaporized around 130oC and then, the decomposition of acetate started around 300oC and finished before 500oC. Therefore, we decided that the temperature and time for preheating was 400oC and 4hours to decompose the acetate fully and then form the layered oxide.
0 20 40 60 80 100
0 200 400 600 800 1000
-120 -80 -40 0 40 80 120
Figure 1. TGA of the mixture of precursors in air.
10 20 30 40 50 60 70 80 90
(a) (b) (c)
105 107 108 110 113
Figure 2. X-ray diffraction patterns of LiNi1/3Co1/3Mn1/3O2 compounds prepared by (a) spray-drying
The powder XRD patterns of LiNi1/3Co1/3Mn1/3O2 compounds prepared from different synthetic methods are shown in Fig. 2. All the prepared materials could be identified as α-NaFeO2 structures with a space group of R¯3m. This was determined by the fact that all of the XRD patterns accorded well with a typical hexagonal pattern and showed a clear split between (108) and (110) peaks.  Table 1 shows the lattice parameters and the unit cell volume calculated from the XRD results. The lattice parameters, a = 2.8602Å and c = 14.2239Å, and the unit cell volume, V = 100.77Å3, of LiNi1/3Co1/3Mn1/3O2 powder (SD) are very consistent with the values reported by Ohzuku.1,7 Other materials (CB and SD) show a slightly lower value.
Table 1. Lattice parameter, mean particle size of the materials prepared from different method.
Method a(Å) c(Å) c/a V(Å3) Mean particle
SD 2.8602 14.2239 4.97 100.77 0.95
CB 2.8532 14.2210 4.98 100.26 1.03
SS 2.8560 14.2204 4.98 100.45 1.14
Samplea 2.862 14.227 4.97 100.91 NA
aN. Yabuuchi, T. Ohzuku,
J. Power Sources, 119-121 (2003) 171
Figure 3. SEM images of LiNi1/3Co1/3Mn1/3O2 powders prepared by (a) spray-drying method, (b)
Fig. 3 shows SEM images ofLiNi1/3Co1/3Mn1/3O2 powders. Although the particle morphology is not clearly shown, all the images show the large agglomeration of small particle with a size of ~1
µm. The particle size distribution in Fig. 4 shows that two of the powders (SD and CB) have a more uniform size distribution in the range of 0.2 to 3 µm than that with a broad distribution (SS) from 0.2 to 10 µm . However, Table 1 shows very similar mean particle size for all three materials.
0 1 2 3 4 5 6 7 8 9
0.1 1 10 100
Particle size (µm)
rticle size distribu
Spray-drying Combustion Solid state reaction
Figure 4. Particle size distribution of LiNi1/3Co1/3Mn1/3O2 powders
Fig. 5 shows the initial charge and discharge curves ofLiNi1/3Co1/3Mn1/3O2 electrodes at 6.0 mA/g in the range from 2.8 to 4.3 V at 25oC. LiNi1/3Co1/3Mn1/3O2 electrodes (SD, CB and SS) show the initial charge/discharge capacities of 171/139 (~81% of coulombic efficiency), 170/128 (~75% of coulombic efficiency) and 174/134 mAh/g (~79% of coulombic efficiency), respectively. All of the materials were prepared from different methods shown by a very similar initial capacity. However, the irreversible capacity observed in the first cycle was about 30-40 mAh/g which is slightly higher than that reported by Ohzuku.1 The dQ/dV plots of LiNi1/3Co1/3Mn1/3O2 electrodes in Fig. 5 (d) show one redox peak at 3.6-3.8V. Ohzuku’s group and Chang’s group proposed that the Ni2+/Ni4+ couple occurs at 3.7-4.0V and the oxidation of Co3+ to Co4+ follows above 4.5V.8, 9
mA/g) and 25oC. The LiNi1/3Co1/3Mn1/3O2 cells showed very similar cycleability up to 4.5V of charging voltage. From 4.6V, the electrode (SS) showed faster capacity fading rather than those (SD and CB). The discharge capacity (SD) showed slightly higher than that (CB).
2.6 2.8 3 3.2 3.4 3.6 3.8 4 4.2 4.4
0 20 40 60 80 100 120 140 160 180
Specific capacity (mAh/g)
(a) Spray-drying (b) Combustion
(c) Solid-state reaction b c a
-400 -200 0 200 400 600 800
3.2 3.4 3.6 3.8 4 4.2
E vs Li/Li+ (V)
(d) (a) Spray-drying
(b) Combustion (c) Solid-state reaction
Figure 5. Initial charge/discharge curves of differential LiNi1/3Co1/3Mn1/3O2 electrodes prepared by (a)
Figure 6. Discharge capacity curves at different discharge rates at C/5, C/2, 1C, 2C, 5C for the
LiNi1/3Co1/3Mn1/3O2 electrodes ranging from 2.8 to 4.3 V.
ic capacity (mAh/g)
Solid state reaction
LiNi1/3Co1/3Mn1/3O2 materials were synthesized from three different methods; spray-drying, combustion, and solid-state reaction. The results from XRD showed that the crystal structure of all the powders was hexagonal structure and the unit cell volume was different according to the synthetic method used. The SEM and particle size analysis of the prepared materials showed uniform size distribution around ~1 µm. The LiNi1/3Co1/3Mn1/3O2 electrodes delivered a discharge capacity of ca. 130-140 mAh/g between 2.8 and 4.6 V and showed good cycleability until the charge voltage reached to 4.6 V. It was found that the LiNi1/3Co1/3Mn1/3O2 material prepared through the spray-drying method showed the largest unit cell volume and better cycleability over those obtained from the combustion and solid-state reaction methods.
This work was financially supported by the Korea Research Foundation Grant funded by the Korean Government (MOEHRD) (KRF-2006-511-D00107).
1. N. Yabuuchi, T. Ohzuku, J. Power Sources 119-121 (2003) 171
2. N. Yabuuchi, Y. Makimura, T. Ohzuku, J. Electrochem. Soc 154 (2007) 314 3. Y.M. Hon, S.P. Lin, K.Z. Fung, M.H. Hon, J. Eur. Ceram. Soc 22 (2002) 653
4. S.H. Park, C.S. Yoon, S.G. Kang, H.-S. Kim, S.-I. Moon, Y.-K. Sun, Electrochim. Acta 49 (2004) 557
5. H.J. Bang, V.S. Donepudi, J Prakash, Electrochim. Acta 48 (2002) 443 6. J.-M. Kim, N. Kumagai, S. Komaba, Electrochim. Acta 52 (2006) 1483 7. I. Belharouak, Y.-K. Sun, J. Liu, K. Amine, J. Power Sources 123 (2003) 247 8. N. Yabuuchi, Y. Makimura, T. Ohzuku, J. Electrochem. Soc. 154 (2007) A314
9. Y.J. Shin, W.-J. Choi, Y.-S. Hong, S. Yoon, K.S. Ryu, S.H. Chang, Solid State Ionics 177 (2006) 515